Research Article  Open Access
V. M. Sounthararajan, A. Sivakumar, "The Effect of Accelerators and Mix Constituents on the High Early Strength Concrete Properties", International Scholarly Research Notices, vol. 2012, Article ID 103534, 7 pages, 2012. https://doi.org/10.5402/2012/103534
The Effect of Accelerators and Mix Constituents on the High Early Strength Concrete Properties
Abstract
The present research study focused on the high early strength concrete properties that can be produced with large replacement of cement by fly ash. Also, the effects of adding fibres on the compressive strength gain and early age strength gain properties are determined. Tests were conducted on different high strength concrete specimens, where fly ash was substituted for cement up to 50%. Different types of concrete specimens were casted and tested for different finetocoarse aggregate ratio, metallic fibre content, cementtototalaggregate ratio, and accelerator dosage. The test results indicated that high early strength concrete (50.7 MPa at 7 days) was obtained for higher F/C ratio of 0.8, C/TA ratio of 0.24, and higher dosage level of steel fibre at 1.5%.
1. Introduction
Highearlystrengthbased cementitious materials are of vital importance for the present expanding civil infrastructure. However, the deterioration of civil infrastructure all over the world has led to the realization that cementitious materials must be improved in terms of their engineering property and durability. The use of admixtures such as fly ash has little effect on pozzolanic properties to improve the engineering properties of flyashsubstituted concrete. In a structural concrete durability should be high, as presented by watertobinder ratio (W/B). A concrete structure is said to be durable if it withstands the conditions for which it has been designed, without deterioration for the entire period of life [1–5]. However, use of chlorides may cause corrosion in steel reinforcing and is prohibited in some countries, so that calcium nitrates can be potentially used to achieve high early strength concrete. These techniques are especially useful in the prefabrication industry, wherein high early age strength enables the removal of the formwork within 24 hours, thereby reducing the cycle time, resulting in costsaving benefits [6]. Pozzolana increases the later age strength of concrete as it reacts with calcium hydroxide and turns it into calciumsilicatehydrates (CSH). However, Portland pozzolana cements have higher activation energy and, therefore, their rate of hydration is lower as compared to ordinary Portland cements [7]. In a similar context, the addition of steel fibers improves the concrete matrix in all mechanical properties of concrete such as compressive strength, spilt tensile strength, flexural strength, and toughness. Steelfiberreinforced concrete is made for cementbased composite material reinforced with randomly distributed steel fibers diameter. It contains pozzolans and admixtures commonly used in pavement construction in civil works [8]. In this similar area of research, it can be observed from earlier studies that the durability properties of concrete is not affected in the case of high early age strength gain in concrete [9]. Also, the addition of mineral and chemical admixtures contributed towards the increase in the rate of strength gain and showed an improvement in the 1 day compressive strength upto 30 MPa which can be sufficient for early removal of formwork [10, 11]. It can be noted that both compressive strength and UPV of all the samples increased especially for samples containing fly ash. The relationship between UPV and compressive strength was found to be exponential for mineral admixtures [12]. The nondestructive testing using ultrasonic testing technique was further extended to study the steelfiberreinforced cementitious materials to predict the influence of volume fraction and fibre geometry on the engineering properties of concrete. The present study is aimed at exploring the strength characteristics of cementitious system, containing steel fibers, fly ash, and accelerator at different dosages. Also, the rate of hardening was monitored using a portable ultrasonic pulse velocity tester.
2. Materials and Experimental Methods
Ordinary Portland cement of 53 grade having 28day compressive strength of 54.9 MPa, satisfying the requirements of IS: 122691987 was used. The specific gravity of cement was found to be 3.12. Fine aggregates obtained from locally available river sand passing through 4.75 mm IS sieve conforming to grading zone II of IS: 3831978 was used. It has fineness modulus of 2.60, a specific gravity of 2.69, and water absorption of 0.97% at 24 hours. Coarse aggregates of crushed blue granite stone with 12.5 mm maximum size conforming to IS: 3831978 was used. The specific gravity was found to be 2.75, fineness modulus 6.5, and water absorption 0.62% at 24 hours. A sulphonated naphthalene formaldehyde based superpalsticizer was used in the study which conforms to ASTM type F and IS: 91031999. Specific gravity of SNF was 1.20. Fibers conforming to ASTM A82001 were used, end hooked steel fibers were used at dosage levels of 0.5 and 1.5% by volume fraction of concrete, the diameter of steel fibres was 0.5 mm, length was 30 mm and its aspect ratio (l/d) of 60, ultimate tensile strength was 900 MPa, and elastic modulus was 210 GPa. An accelerator was used to obtain a high early strength concrete at dosage level of 1% by weight of cement. The concrete mixture proportions used in the study are provided in Table 1. The total 16 different concrete mixtures were proportioned based on the cementtototalaggregate ratio (C/TA) 0.24 and 0.26, watertocement ratio (W/C) 0.3 and 0.4, and finetocoarseaggregate ratio (F/C) 0.6 and 0.8. The concrete mixtures were mixed using a 40liter container with tilting drum type mixer, and specimens were cast using steel mould, the standard cube (100 × 100 × 100 mm) moulds, and cylinders (100 mm diameter × 200 mm height) and compacted with table vibrator. For each mix at least three specimens were remoulded 24 hours after casting and watercured at °C until the age of testing of 1, 3, 7, 14, 28, and 56 days. All the specimens were cured in the same curing tank to maintain uniform curing for all the specimens.

3. Experimental Test Results and Discussions
The compressive test results of different concrete mixtures are given in Tables 2 and 3 and shown in Figures 1, 2, 3, 4, and 5. It can be observed that compared to control concrete all the concrete composites containing metallic fibre content showed higher strength. It can also be noted that the variables such as cementtoaggregateratio and fine to coarseaggregateratio affected the compressive properties greatly when the W/C ratio was 0.3 as observed in Figure 1. Similarly it can be seen from Figures 2 and 5, that compared to 0.3 W/C ratio, 0.4 W/C showed higher strength due to higher F/C (0.8) ratio, whereas the C/TA (0.24) was lower than the lower W/C (0.3) ratio. Also, the same trend was observed for the controlled concrete mix, which resulted in marginal increase in the compressive strength for W/C and C/TA ratio. Also it is well noted that higher F/C ratio used in concrete resulted in higher strength. This can be justified based on the fact that both the parameters C/TA and F/C ratio have significant effect on the improvement the rate of strength gain (as observed in Figures 6, 7, 8, and 9). This can lead to delayed cracking in concrete upon loading. The split tensile properties further showed similar trend as that of compressive strength. The test results on the early age hardening in few hours after demoulding the concrete specimens were recorded and are shown in Table 4. The ultrasonic test results values showed that the strength gain after 1 day exhibited a good increase in pulse velocity and satisfied the IS 13311 (shown in Figure 10). This essentially shows that the good quality concrete was obtained at much earlier period of curing with the addition of accelerator and fibres.



4. Conclusions
Based on the above experimental investigation, the following conclusions can be drawn. (i)The use of class F flyash and accelerator showed that early age setting properties of concrete can be more useful where high early fast track concreting is required. Also, the addition of metallic content has significant effect on the compressive and split tensile properties of concrete. (ii)The careful selection of different variables such as cementtoaggregateratio and fine to coarseaggregateratio has significant effect as well as cementtoaggregateratio which provided greater improvements in the mechanical properties of concrete.(iii)It is clearly evident that early strength gain in concrete is a function of low watercementratio, F/C ratio, accelerator dosage, and cementtototalaggregate ratio. Cement replacement up to 50% fly ash showed early age strength gain slightly lower than concrete made with 25% fly ash. Therefore, concrete mixes containing class F ash can be used up to 50% safely to produce high early strength concrete for precast products.(iv)It was observed from the test results that the higher strength was obtained for W/C ratio 0.3, F/C ratio 0.8, and C/TA ratio 0.24 with metallic content 1.5% from which the compressive strength at 28 days was 54.9 MPa and a similar trend was noted for lower W/C ratio of 0.3, F/C ratio 0.6, and C/TA ratio 0.26 with higher metallic content 1.5% from which the test result value for 28 days was 53.4 MPa. It can be concluded that higher finetocoarseaggregates ratio and metallic fiber content up to 1.5% showed higher strength. The addition of accelerator has direct effect on the early strength gain and resulted in attaining the 28 days in a short duration of 7 days.
References
 T. R. Naik and B. W. Ramme, “Low cement content high strength concrete,” Cement and Concrete Research, vol. 17, no. 2, pp. 283–294, 1987. View at: Google Scholar
 K. Ganesh Babu and G. Siva Nageswara Rao, “Efficiency of fly ash in concrete with age,” Cement and Concrete Research, vol. 26, no. 3, pp. 465–474, 1996. View at: Google Scholar
 BIS (Bureau of Indian Standards), “Specification for 53grade Ordinary Portland cement,” IS 122691987, New Delhi, India, 1987. View at: Google Scholar
 BIS (Bureau of Indian Standards), “Nondestructive testing of concrete Part 1 Ultrasonic pulse velocity,” IS 133111992, New Delhi, India, 1992. View at: Google Scholar
 ACI Committee 544, “Guide for specifying, mixing, placing and finishing steel fiber reinforced concrete,” ACI 544. 3R 95, American Concrete Institute, Detroit, Mich, USA, 2006. View at: Google Scholar
 P. S. Song and S. Hwang, “Mechanical properties of highstrength steel fiberreinforced concrete,” Construction and Building Materials, vol. 18, no. 9, pp. 669–673, 2004. View at: Publisher Site  Google Scholar
 S. R. Parimi and J. K. S. Rao, “Effectiveness of random fibres in fibrereinforced concrete mechanical behaviour of materials,” in Proceeding International Conference on Mechanical Behaviour of Materials, vol. 5, pp. 176–186, 1971. View at: Google Scholar
 P. Rossi, “Mechanical behaviour of metalfibre reinforced concretes,” Cement and Concrete Composites, vol. 14, no. 1, pp. 3–16, 1992. View at: Google Scholar
 A. E. Naaman and H. Hammoud, “Fatigue characteristics of high performance fiberreinforced concrete,” Cement and Concrete Composites, vol. 20, no. 5, pp. 353–363, 1998. View at: Google Scholar
 C. Huang and G. Zhao, “Properties of steel fibre reinforced concrete containing larger coarse aggregate,” Cement and Concrete Composites, vol. 17, no. 3, pp. 199–206, 1995. View at: Google Scholar
 S. M. Mohammed and B. Mohamed, “Properties of concrete reinforced with different kinds of industrial waste fibre materials,” Construction and Building Materials, vol. 23, no. 10, pp. 3196–3205, 2009. View at: Publisher Site  Google Scholar
 J. H. Bungey, “The validity of ultrasonic pulse velocity testing of inplace concrete for strength,” NDT International, vol. 13, no. 6, pp. 296–300, 1980. View at: Google Scholar
Copyright
Copyright © 2012 V. M. Sounthararajan and A. Sivakumar. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.